- Home
- Documents
*MANUAL FOR FATIGUE ANALYSIS OF Abstract The approach for the high-cycle fatigue life prediction of a...*

prev

next

out of 55

View

220Download

6

Embed Size (px)

i

MANUAL FOR FATIGUE ANALYSIS

OF

REINFORCED CONCRETE STRUCTURAL

ELEMENTS USING

VecTor2

Benard Isojeh

Frank Vecchio

December, 2017

ii

Abstract

The approach for the high-cycle fatigue life prediction of a reinforced concrete structural element

using VecTor2 nonlinear finite element analysis is presented. Mechanisms governing fatigue

damage progressions are briefly discussed, and the implementation of the models that account

for these mechanisms in VecTor2 software is treated subsequently. In addition, an illustrative

solution for a single element subjected to shear fatigue loading is given. The VecTor2 nonlinear

finite element analysis software, which incorporates fatigue damage models, allows for the

prediction of the fatigue residual capacity of an element after a given number of loading cycles.

The prediction of the instance at which steel reinforcement will fracture can also be obtained

from the analyses results.

iii

Table of contents

Abstract .... ii

List of Figures....v

Notations..vii

CHAPTER 1: FATIGUE DAMAGE MECHANISMS.....1

1.1 Introduction .....1

1.1.1Strength Degradation...........1

1.1.2 Irreversible Strain Accumulation3

1.1.3 Reinforcement Crack Growth.....4

1.2 Damage Constitutive Models for Residual Strength of Concrete....6

1.2.1 Normal Strength Concrete............................................6

1.2.2 High Strength Concrete8

CHAPTER 2: IMPLEMENTATION OF DAMAGE MODELS IN DSFM.....9

2.1 Disturbed Stress Field Model.......9

2.1.1 Equilibrium Conditions....9

2.1.1.1 Equilibrium of Stresses at a Crack.....10

2.1.2 Compatibility Condition.12

2.1.3 Constitutive Relation...13

2.1.3.1 Concrete Constitutive Model..13

2.1.3.2 Conventional Reinforcement..17

CHAPTER 3: FINITE ELEMENT IMPLEMENTATION.....18

3.1 Formulation18

iv

3.2 Failure Criterion for Reinforced Concrete and Steel-Fibre Concrete under Fatigue

Loading22

3.3 Solution for Fatigue Loading at 10 000 cycles......24

CHAPTER 4: USE OF VecTor2 FOR FATIGUE DAMAGE ANALYSIS...30

4.1 Defining Concrete Materials.30

4.2 Defining Reinforcement Properties...31

4.3 Bond Types...32

4.4 Structure and Mesh Definition..33

4.5 Load Application under Fatigue Loading..33

4.6 Job Definition....34

4.7 Defining Fatigue Loading Parameters in Job....36

4.8 Solved Example.....38

5.0 SUMMARY AND RECOMMENDATION..41

5.1 Summary41

5.2 Recommendation...41

6.0 REFERENCES......42

v

List of Figures

CHAPTER 1: FATIGUE DAMAGE MECHANISMS

Fig. 1.1 Estimation of damage parameter s...2

Fig. 1.2 Crack growth on a reinforcing bar cross section5

Fig. 1.3 - Modified Stress-strain curve for damaged concrete...7

CHAPTER 2: IMPLEMENTATION OF DAMAGE MODELS IN DSFM

Fig. 2.1 Reinforced concrete element.10

Fig. 2.2 Equilibrium conditions.....11

Fig. 2.3 - Equilibrium conditions along crack surface after reinforcement crack propagation11

Fig. 2.4 - Damage parameter s for steel fibre secant modulus (A) and residual strength (B)..14

CHAPTER 3: FINITE ELEMENT IMPLEMENTATION

Fig. 3.1 - Flow chart for the modified solution algorithm for DSFM......21

Fig. 3.2 - Shear panel (PV19)..23

Fig. 3.3 - Crack slip evolution.....28

Fig. 3.4 - Shear stress evolution at crack.....28

Fig. 3.5 - Reinforcement (Y-direction) crack growth depth28

Fig. 3.6 - Reinforcement (X-direction) strain evolution at crack location..29

Fig. 3.7 - Reinforcement (X-direction) average stress evolution....29

Fig. 3.8 - Localised reinforcement strain evolution (Ydirection)..29

CHAPTER 4: USE OF VecTor2 FOR FATIGUE DAMAGE ANLYSIS

Figure 4.1- Formwork application window.....30

Figure 4.2 Reinforced concrete materials properties dialog box..31

Fig. 4.3 Reinforcement materials dialog box........32

vi

Figure 4.4 Bond properties dialogue box.32

Figure 4.5 Structure and mesh definition..33

Fig. 4.6 Fatigue load wave form (sinusoidal)...34

Figure 4.7 Load application..34

Figure 4.8 Job control...35

Fig. 4.9 Concrete models..36

4.10 Fatigue damage consideration..37

Fig. 4.11 Fatigue damage parameters...37

Fig. 4.12 - Details of deep beam specimen.....38

Fig. 4.13 Finite element mesh for beam...39

Fig. 4.14 Load versus mid-span deflection..40

Fig. 4.15 Fatigue residual capacity..40

Fig. 4.16 Mid-span deflection evolution..41

Fig. 4.17 Evolution of stresses in reinforcing bars (stresses shown in MPa)...41

vii

Notation

The following symbols are used (may not be defined in the text):

a,b,c : material parameters

C: material constant = 2 x 1013

: frequency factor

D : damage

: rebar diameter

: concrete stiffness matrix

: critical damage

: concrete tensile strength damage

: reinforcement stiffness matrix

: concrete tensile secant modulus damage

: elastic modulus of concrete

1: secant modulus of concrete in tension

2: secant modulus of concrete in compression

: elastic modulus of steel reinforcement

: shear modulus

f : frequency

1: effective tensile stress of concrete

2: effective compressive stress of concrete

,: average tensile stress in concrete due to tension stiffening effect

: normal stress in concrete in horizontal direction

: normal stress in concrete in vertical direction

viii

: shear stress in concrete in horizontal direction

2: peak compressive stress in concrete considering compression softening effect

: tensile stress due to mechanical anchorage effect of end-hooked steel-fibre

: tensile stress at crack due to steel fibre

: initial compressive strength

: tensile stress due to frictional bond behaviour of steel fibre

: initial concrete tensile strength

: compressive strength of concrete

fc: degraded compressive strength

: local stress in reinforcement at crack

: average stress in steel reinforcement

: residual tensile strength of concrete

: degraded strength at which concrete cracks

k: post-decay parameter for stress-strain response of concrete in compression

N : number of cycles

n: curve-fitting parameter for stress-strain response of concrete in compression

n: material constant = 3

: numbers of cycles at failure

: interval of cycles considered

: crack spacing

: period of fatigue cycle

: direction coefficient (= 0.6 or 1.0)

v: Poissons ratio

ix

vci : shear stress

vci,cr : shear stress at cracked concrete plane

Vf: steel fibre volume ratio

: crack width

: coefficient to relate tensile stress at a crack due to steel fibres with average tensile stress

: inclination of reinforcement

: material constant

2 : material constant

: deformation

1: change in strain at crack

: fatigue stress

: crack slip

1: net tensile strain

2 : net compressive strain

: strain corresponding to the degraded compressive strength

: local strain in the reinforcement

: average strain in steel reinforcement

: irreversible fatigue strain

: initial strain corresponding to the initial compressive strength

1: local strain at crack

2: parameter for high stress level

: shear strain due to crack slip

, c : inclination of principal strain direction

x

: angle between the reinforcement direction and the normal to the crack

: reinforcement ratio

1

CHAPTER 1: FATIGUE DAMAGE MECHANISMS

1.1 Introduction

The fatigue loading of a reinforced concrete element is well-known to result in a progressive

deterioration of concrete. Once concrete cracking occurs, reinforcement crack propagation at the

intersection with the cracked concrete planes may occur depending on the magnitude of the

induced stress in the steel reinforcement. However, robust models required for predicting the

fatigue life of these elements are not readily available. This is attributable to the complex

degradation mechanisms for steel and concrete composites inherent in any fatigue damage process

(Isojeh et al., 2017e).

To fully account for fatigue damage mechanisms, concrete integrity deterioration, irreversible

strain accumulation, and reinforcement crack growth should be considered. Herein, the mechanism

are incorporated into the constitutive, compatibility and equilibrium equations of the Disturbed

Stress Field Model (DSFM) (Vecchio, 2000) analysis algorithm to predict the fatigue residual

capacity of a structural element. The fatigue life of a structural element corresponds to the instance

when the fatigue residual capacity becomes equal to the applied fatigue load (Isojeh et al., 2017e).

The damage mechanisms are considered subsequently.

1.1.1 Strength Degradation

Results of the investigations reported in the literature have shown that concrete strength and

stiffness reduce progressively after fatigue loading cycles have been a